Chemical-Mechanical Polishing: Enhancing the ...
Embed Size (px)
Transcript of Chemical-Mechanical Polishing: Enhancing the ...
Chemical-mechanical polishing: enhancing the manufacturability of MEMS
Jeffry J. Sniegowski
Intelligent Micromachines DepartmentSandia National Laboratories, Albuquerque, NM 87185
The planarization technology of Chemical-Mechanical-Polishing (CMP), used for the manufacturing of multi-level
metal interconnects for high-density Integrated Circuits (IC), is also readily adaptable as an enabling technology in
MicroElectroMechanical Systems (MEMS) fabrication, particularly polysilicon surface micromachining. CMP not
only eases the design and manufacturability of MEMS devices by eliminating several photolithographic and film issues
generated by severe topography, but also enables far greater flexibility with process complexity and associated designs.
Thus, the CMP planarization technique alleviates processing problems associated with fabrication of multi-level
polysilicon structures, eliminates design constraints linked with non-planar topography, and provides an avenue for
integrating different process technologies. Examples of these enhancements include: an simpler extension of surface
micromachining fabrication to multiple mechanical layers, a novel method of monolithic integration of electronics and
MEMS, and a novel combination of bulk and surface micromachining.
Keywords: surface micromachining, polysilicon, microelectromechanical systems, chemical mechanical polishing,
The intent of this paper is to overview the benefits of wafer planarization by chemical-mechanical-polishing (CMP)
for MicroElectroMechanical Systems MEMS fabrication. CMP is readily adapted to the MEMS fabrication
technology known as polysilicon surface micromachining. A brief description of CMP process technology followed by
a cursory description of polysilicon surface micromachining clearly illustrate why CMP is compatible and how surface
micromachining benefits from this technology. We then provide several examples of how CMP enhances the
manufacturability of a standard, non-planarized surface micromachining process. The final sections discuss new design
and process directions enabled through the use of CMP planarization.
2. CHEMICAL-MECHANICAL POLISHING
CMP processes produce both global and local planarization through relatively simple and quick processing. Figure
1 illustrates the CMP process in which an oxide surface is planarized by rotating a wafer under pressure against a
polishing pad in the presence of a silica-based alkaline slurry. The theory of oxide polishing is not well understood,
however, it is generally accepted that the alkaline chemistry hydrolyzes the oxide surface and sub-surface thusweakening the SiO2 bond structure1. The mechanical energy imparted to the abrasive slurry particle through pressure
and rotation causes high features to erode at a faster rate than low features, thereby planarizing the surface over time.
For the particular results shown here, a colloidal-fumed silica slurry (Cabot SS-12) and a polyurethane pad (Rodel
IC1000/Suba IV) are used.
Fig. 1 Schematic representation of CMP process in which an oxide surface is planarized by rotating the waferunder pressure against a polishing pad in the presence of a silica-based alkaline slurry.
Fig. 2 SEM cross-section of a partially-fabricated micromachine illustrating the uneven, severe topographybefore CMP planarization.
Fig. 3 SEM cross-section of a partially-fabricated micromachine after CMP planarization. Note theplanarity of the upper oxide surface.
One of the main differences between planarizing inter-level dielectric materials used in ULSI interconnect
technology and planarizing sacrificial oxide material used in MEMS technology is the large step heights (2-4 µm vs.
0.8 µm) associated with polysilicon surface micromachined MEMS. These large step heights present a challenge to
any planarization strategy. Figures 2 and 3 show the surface topography of single level polysilicon structure prior to
CMP (2) and after the CMP process (3). As can be seen from the figures, CMP does an excellent job of removing the
~ 2 µm step height and planarizing the oxide surface.
2. ENHANCED MANUFACTURABLILITY OF SURFACE MICROMACHINED MEMS
MEMS process technologies, and in particular polysilicon surface micromachining2,3, have been plagued by
process issues generated by severe vertical topography which is introduced by the repetitive deposition and etching of
multiple films. Polysilicon surface micromachining readily adapts to the inclusion of CMP and clearly illustrates the
benefits of CMP for several reasons. Surface micromachining uses the planar fabrication techniques and films common
to the microelectronic circuit fabrication industry to manufacture micromechanical devices. The standard building-
block process consists of depositing and photolithographically patterning alternate layers of low-stress polycrystalline
silicon and sacrificial silicon dioxide. The result is a construction system consisting of one layer of polysilicon which
provides electrical interconnection and one or more independent layers of mechanical polysilicon which can be used to
form mechanical elements ranging from simple cantilevered beams to complex systems of springs, linkages, mass
elements and joints. At the completion of the process, the sacrificial layers, as their name suggests, are selectively
etched away in hydrofluoric acid (HF), which leaves the free-standing polysilicon layers. Figure 4 illustrates both the
essence of polysilicon surface micromachining and clearly displays the vertical topography which arises during the non-
planarized process. This topography can produce mechanical interference between moving parts, and complicates
subsequent process steps.
Fig. 4 Focused Ion Beam (FIB) milled cross-section of a mechanical joint formed in a three-layer polysiliconsurface micromachining technology2. The final mechanical polysilicon film is the upper light-colored filmwhich illustrates the topography and the interference artifacts generated (arrows) by the previous film steps.The film thicknesses are on the order of 2µm for both the mechanical polysilicon films and the sacrificialsilicon dioxide films.
The mechanical interference arises when an upper layer of polysilicon must pass over the edge of a previously
etched lower layer. An example of this interference, taken from the microengine3, can be seen in Fig. 5a where the
upper link runs over the edge of the gear causing an overhang feature. This feature is due to the conformal deposition
of the polysilicon film. Link/gear interference can be alleviated by the microengine design, or by planarization of the
surfaces before subsequent deposition of additional films as illustrated in the CMP-planarized joint in Fig. 5b.
l i nkagearm
planarizedl i nkage arm
Fig. 5 The SEM Fig. 5a illustrates the artifacts generated by the conformal nature of the polysilicondepositions over prior topology (indicated by arrows), while Fig. 5b illustrates the same microengine jointfeature fabricated with planarization by CMP before the final polysilicon deposition. The overhang artifactsare no longer present.
In addition to the above design constraint, two significant process difficulties arise from severe topography. The
first results from the use of highly anisotropic plasma etch processes for the definition of the polysilicon layers. The
anisotropy is necessary to obtain the desired vertical sidewalls of the polysilicon structures. However, the very
anisotropy of the etch also prevents the etch from removing the polysilicon layer from along the edge of a step. This
produces long slivers of polysilicon, often referred to as stringers, along these edges as illustrated in Fig. 6. The
stringers can also produce mechanical interference or even an electrical short. Secondly, photolithographic definition of
subsequent layers becomes problematic over severe topography. Photoresist, the photosensitive polymeric coating used
to transfer the design into the physical films, becomes difficult to apply, expose, and develop, leading to loss of
resolution and definition. Removal of these difficulties through the use of CMP aids manufacturability by reducing or
eliminating photolithography reworks.
Fig. 6. Polysilicon stringer next to a gear edge. The stringer was formed during a later polysilicondeposition and patterning.
Thus, the addition of chemical-mechanical polishing (CMP) planarization to polysilicon surface micromachining
technology is a major process enhancement from both the process and design perspectives4. Techniques other than
CMP for overcoming topography problems have also been used by researchers in the MEMS community. For
example, researchers at University of Wisconsin have demonstrated locally-planarized surface-micromachined pressure
sensors produced in a double LOCOS process5; while the use of plasma planarization has recently been demonstrated
on MEMS devices by researchers at Delft6. Although these planarization techniques have yielded improvement in the
manufacturability of MEMS devices through local planarization, CMP provides a higher quality of both local and
global planarization in a manufacturing environment. CMP, best known for its global planarization use in sub-micron
circuit technology7, was first used in the MEMS field to improve the optical quality of polysilicon surface-
micromachined mirror devices by smoothing the polysilicon8. However, the first use of CMP planarization in MEMS
was reported by Sniegowski4,9 in the application of a three-level polysilicon process for the microengine.
The benefits of CMP for surface-micromachining are four-fold. It eliminates the potential mechanical interference
problem. It eliminates the artifact of anisotropic etching of conformal polysilicon films over edges, i.e. stringers, since
there are no edges on a planar surface. Thirdly, the extension to four or more levels of polysilicon becomes practical
since the topography and associated photolithographic problems are eliminated. Finally, CMP planarization provides
an avenue to integrate separate process technologies such as microelectronics and micromechanics or surface
micromachining and high-aspect-ratio micromachining. The first three benefits combine to produce higher device yield
and reliability, while the latter two combine to produce exciting new processes and designs as described in section 3.
3. ADVANCED MEMS APPLICATIONS OF CMP
The previous section dealt primarily with improved manufacturability of MEMS with large topography. This
section continues to illustrate enhancements to manufacturing, but principally describes new capabilities made possible
3.1 Multi-Level Structures
Multiple levels of structural polysilicon enable fabrication of increasingly complex MEMS devices such as
microengines10 capable of driving sets of gears. Simple flexure structures such as comb drives11 can be built in a single
level of structural polysilicon while a second level enables the production of gears with pin joints. A third level enables
linkages between spinning gears, but introduces severe topography problems that must be solved with a combination of
careful process and device design or solved by planarization with CMP as previously described in section 2, Fig. 5.
Figure 7 shows a geared transmission unit with multi-level, compound gears. Although designed to accommodate non-
planar processing (as made apparent by the etch artifacts seen on the surface of the top large gear), the design was
actually fabricated with CMP to produce fully functional units. A new design, not compromised with the non-planar
design, will lend itself to more reliable operation.
Fig. 7 is an SEM of the completed gear-speed-reduction unit and linear rack. The linear speed of the rack isapproximately one tenth that of the linear tooth velocity of the drive gear. The rack has been successfullyused to drive a folding mirror, for example.
Additional levels of polysilicon promise even more complex structures, but the extreme topography of these multi-
level structures (four or more active layers) has prohibited their fabrication. A micromachining technology that
includes planarization steps such as CMP will enable device fabrication with these additional levels.
3.2 Pressure Sensors
A planar pressure sensor technology12 has been developed based upon a silicon nitride layer as the diaphragm
material. A trench is etched ~2 µm deep in the surface of a silicon wafer. This trench is refilled with a sacrificial oxide
and planarized with CMP. A silicon nitride diaphragm layer is then deposited. The sacrificial oxide underneath this
diaphragm layer is removed using HF leaving a cavity beneath the diaphragm. An additional silicon nitride layer is
used to seal the cavity in near-vacuum conditions (approx. 200 mTorr). Polysilicon piezoresistors are deposited on the
diaphragm to sense the diaphragm strain that results from changes in ambient pressure. A completed, 100-µm-diameter
planar pressure sensor is shown in Fig. 8. This sensor shows marked improvement in planarity when contrasted against
a similar, non-planar sensor shown in Fig. 9.
Fig. 8. Top view of a planar pressure sensor fabricated in a process that includes CMP. The reference cavityis embedded below the substrate surface, eliminating step coverage problems.
Fig. 9. Top view of a non-planar pressure sensor. The circular diaphragm covers a 2µm-high referencevacuum cavity, and is the source of step coverage problems.
In the non-planar sensor manufactured without CMP the reference pressure cavity is formed above the silicon
surface producing large step heights. These steps cause processing difficulties with photoresist coverage and removal,
dry etch selectivity to photoresist where the photoresist thins over steps, and metal step coverage. These challenges to
manufacturing were eliminated in the CMP-planarized sensor. In the future, the use of an embedded cavity will enable
the monolithic integration of this sensor technology with CMOS in a modified version of the integration process
described later in this paper, and will also enable the use of deeper vacuum cavities to extend the sensing range of the
Fig. 10. Cross-section of a high-aspect-ratio polysilicon accelerometer proof mass with CMP-planarized topsurface.
Fig. 11. Cross-section of a high-aspect-ratio tungsten accelerometer proof mass with CMP-planarized topsurface.
3.3 High-Aspect Ratio Micromachining
In addition to its uses for planarization of surface-micromachined devices, CMP plays a key role in the fabrication
of high-aspect ratio micromolded polysilicon and tungsten devices. In the technology presented here13, deep, narrow
trenches lined with oxide are filled with thin films (~2-5 µm) of either polysilicon as shown in Fig. 10 or tungsten as
shown in Fig. 11 and planarized with CMP. These structures can then be integrated with surface micromachined
polysilicon structures to form large high-aspect-ratio proof masses with compliant surface-micromachined springs as
shown in Fig. 12.
Fig. 12. High-aspect-ratio polysilicon accelerometer mass integrated with a surface-micromachined spring.
3.4 Integration of MEMS with Microelectronics
Recently, a great deal of interest has developed in manufacturing processes that allow the monolithic integration of
MEMS with driving, controlling, and signal processing electronics14. The monolithic integration of micromachines and
microelectronics enables the development of wide new classes of small, smart, products with maximum levels of system
performance. A new integration scheme15 overcomes the limitations of traditional integration schemes and enables, for
the first time, the integration of micromachines of arbitrary complexity with high performance, state-of-the-art CMOS.
Functionality yields in excess of 98% have been achieved with this technology16. An example of devices built in this
technology are shown in Fig. 13.
Fig. 13. Surface-micromachined polysilicon resonators built in a trench alongside their CMOS sensingelectronics.
We have developed this embedded MEMS approach to enhance the manufacturability, design flexibility, and
performance of microelectronic/micromechanical devices. This process places the micromechanical devices in a
shallow (~6-12 µm) trench, planarizes the wafer, and seals the micromechanical devices in the trench. These wafers
with the completed, planarized micromechanical devices are then used as starting material for a conventional CMOS
process. This technique is equally applicable to other microelectronic device technologies such as bipolar or BiCMOS.
Since this integration approach does not modify the CMOS processing flow, the wafers with the subsurface
micromechanical devices can also be sent to a foundry for microelectronic processing. Furthermore, the topography of
multiple polysilicon layers does not complicate subsequent photolithography. A high-temperature anneal is performed
after the devices are embedded in the trench prior to microelectronics processing. This anneal stress-relieves the
micromechanical polysilicon and ensures that the subsequent thermal budget of the microelectronic processing does not
affect the mechanical properties of the polysilicon structures.
Fig. 14 is a schematic cross-section of the integrated technology. Alignment marks are etched onto the surface of
wafer in order to provide reference locations for subsequent processing. A shallow trench is etched in (100) silicon
wafers using an anisotropic etchant that preferentially etches the (100) crystal plane and produces a trench with
sidewalls having a slope of 54.7° relative to the surface. This slope aids in the subsequent photo patterning within the
Figure 15. Cross-sectional schematic of the subsurface, embedded MEMS integrated technology.
The alignment marks from the top surface of the wafer are used as references to generate another set of alignment
marks on the bottom surface of the trench. This approach is used to optimize level-to-level registration and resolution
of features within the trench. Feature sizes with critical dimensions as small as 0.8 µm, the limit of g-line lithography,
were successfully defined within the trench.
A silicon nitride film is deposited to form a dielectric layer on the bottom of the trench. Sacrificial oxide and
multiple layers of polysilicon are then deposited and patterned in a standard surface micromachining process.
Polysilicon studs provide contact between the micromechanical devices and the CMOS devices; the depth of the trench
is sized so that the top of the polysilicon stud lies just below the top of the planarized trench. The shallow trenches are
then filled with a series of oxide depositions optimized to eliminate void formation in high-aspect-ratio structures. The
wafer is subsequently planarized with chemical-mechanical polishing (CMP). The entire structure is annealed to relieve
stress in the structural polysilicon and sealed with a silicon nitride cap. At this point, conventional CMOS processing is
performed. The backend of the process requires an additional step to open the nitride cap over the micromechanical
layer prior to release of the micromechanical structures. Photoresist is used as a protection layer over the exposed bond
pads during the release process.
This technology does not impose additional limits on the size, thickness, or number of layers of the
micromechanical polysilicon structures. The modularity of the process allows changes to be made to either the
micromechanical process or the microelectronic process without affecting the other process. A planarized wafer with
the embedded MEMS can serve as starting material for a conventional microelectronics foundry service since the
technology does not require significant modifications of standard microelectronic fabrication processes.
Once the basic chemical-mechanical polishing planarization technique for silicon dioxide over polysilicon is set-up
and developed in a fabrication line, the process is readily adaptable for use in polysilicon surface micromachining.
Although the planarization is a conceptually "simple" step, the impact of its inclusion in the overall fabrication process
is immense. Manufacturing impediments are removed while novel, expanded processes and designs become possible.
CMP increases yield and functionality of many of device design which had previously been processed with a non-
planarized technique. Expanded processes can entail the inclusion of four or more layers of mechanical polysilicon
films for more complex out-of-plane structures. Novel processes such as combining trenched structures with surface-
micromachined structures or monolithic integration of MEMS with circuitry by embedding the MEMS in a planarized
well can be realized. Further, a change in design perspective occurs since the need to circumvent mechanical
interference in a non-planarized process is alleviated. Thus, more complex designs with greater functionality yet
created from simpler stepwise designs are feasible.
We anticipate that CMP planarization, in the next few years, will be used extensively within the MEMS community
for polysilicon surface micromachining. In addition, other MEMS fabrication technologies such as bulk
micromachining and LIGA can potentially benefit from CMP, however CMP may not be as suitable for adaptation to
these technologies as it is to surface micromachining.
This paper discusses the work of many people at the Sandia National Laboratories' Microelectronics Development
Laboratory including C. Apblett (CMP), C. C. Barron (Accelerometers/high-aspect-ratio process), W. Eaton(Pressure
sensor), J. G. Fleming (High-aspect-ratio process), D. Hetherington (CMP), S. Montague (CMOS/MEMS Integration),
R. Nasby (CMP), M. S. Rodgers (Device design/layout), J. Smith (Sensors & CMOS/MEMS Integration), and J.
Sniegowski (Actuators, CMOS/MEMS Integration, & CMP). The process development engineers, operators, and
technicians of the Microelectronics Development Laboratory are also acknowledged for their contributions to the
process development, fabrication, and testing of these devices.
This work, performed at Sandia National Laboratories, was supported by the U. S. Department of Energy under
1 L. Cook, "Chemical processing in glass polishing," J. Non-Cryst. Solids, 120, pp. 152-171, (1990).2 R. T. Howe and R. S. Muller, "Polycrystalline Silicon Micromechanical Beams," J. Electrochem. Soc.:SOLID-STATE
SCIENCE AND TECHNOLOGY, Vol. 103, No. 6, pp. 1420-1423, June 1983.3 J. J. Sniegowski and E. J. Garcia, "Microfabricated actuators and their application to optics", Proc. SPIE Miniaturized
Systems with Micro-Optics and Micromechanics, 2383, 2/7-9/95, San Jose, CA, pp. 46-64, (1995).4 R. D. Nasby, J. J. Sniegowski, J. H. Smith, S. Montague, C. C. Barron, W. P. Eaton, P. J. McWhorter, D. L.
Hetherington, C. A. Apblett, and J. G. Fleming, "Application of chemical-mechanical polishing to planarization ofsurface-micromachined devices", Solid-State Sensor and Actuator Workshop, Hilton Head Is., SC, pp. 48-53, June 3-6,1996.
5 H. Guckel and D. Burns, "Planar Processed Polysilicon Sealed Cavities for Pressure Transducer Arrays," IEDM, pp. 223-225 (1984).
6 Y. Li, P. French, and R. Wolffenbuttel, “Plasma planarization for sensor applications,” IEEE JMEMS, 4, pp. 119-131,(1995).
7 Patrick, W., Guthrie, W., Standley, C., and Schiable, P., 1991, "Application of chemical mechanical polishing to thefabrication of VLSI circuit interconnections," J. Electrochem. Soc., vol. 138, pp. 1778-1784.
8 A. Yasseen, S. Smith, M. Mehregany, and F. Merat, "Diffraction grating scanners using polysilicon micromotors,"Proceedings, IEEE Micro Electro Mechnical Systems Workshop '95, pp. 175-180.
9 J. J. Sniegowski, "Surface micromachined sensors and actuators", Proceedings, Micro-integrated Smart Material andStructures Conference (MISMSC), Society for Experimental Mechanics, Williamsburg, VA,Oct. 11-12, 1995, pp. 31.
10 J. J. Sniegowski, S. M. Miller, G. F. LaVigne, M.S. Rodgers, and P. J. McWhorter, "Monolithic geared-mechanismsdriven by a polysilicon surface-micromachined on-chip electrostatic microengine,", Proceedings, Solid-State Sensor andActuator Workshop, Hilton Head Is., SC, USA, pp. 178-182, June 3-6, 1996.
11 W. Tang, T-C. Nguyen, and R. Howe, “Laterally Driven Polysilicon Resonant Microstructures,” Sensors and Actuators,20, pp. 25-32 (1989).
12 W. Eaton and J. Smith, “Surface-micromachined planar pressure sensor with a sub-surface, embedded reference pressurecavity,” submitted to SPIE Micromachining and Microfabrication (1996).
13 J. Fleming and C. Barron, “Novel silicon fabrication process for high-aspect-ratio micromachined parts,” Proc. SPIEMicromachining and Microfabrication ‘95, 2639, p. 185 (1995).
14 R. Howe, “Polysilicon integrated microsystems: technologies and applications,” Proc. Transducers ’95, pp. 43-46(1995).
15 J. Smith, S. Montague, J. Sniegowski, J. Murray, and P. McWhorter, “Embedded micromechanical devices for themonolithic integration of MEMS with CMOS”, Proc. IEDM ‘ 95, pp. 609-612 (1995).
16 J. Smith, S. Montague, J. Sniegowski, J. Murray, R. Manginell, P. McWhorter, and R. Huber, “Characterization of theembedded micromechanical device approach to the monolithic integration of MEMS with CMOS”, This proceedings,SPIE Micromachinng and Microfabrication ‘96 Symposium, vol. 2879, Ausitn, TX, October 14-15, 1996.